Microstructural Evolution and Solidiï¬cation Behavior .Microstructural Evolution and...
Embed Size (px)
Transcript of Microstructural Evolution and Solidiï¬cation Behavior .Microstructural Evolution and...
Microstructural Evolution and Solidification Behaviorof Al-Mg-Si Alloy in High-Pressure Die Casting
SHOUXUN JI, YUN WANG, D. WATSON, and Z. FAN
Microstructural evolution and solidification behavior of Al-5 wt pct Mg-1.5 wt pct Si-0.6 wt pctMn-0.2 wt pct Ti alloy have been investigated using high-pressure die casting. Solidificationcommences with the formation of primary a-Al phase in the shot sleeve and is completed in thedie cavity. The average size of dendrites and fragmented dendrites of the primary a-Al phaseformed in the shot sleeve is 43 lm, and the globular primary a-Al grains formed inside the diecavity is at a size of 7.5 lm. Solidification inside the die cavity also forms the lamellar Al-Mg2Sieutectic phase and the Fe-rich intermetallics. The size of the eutectic cells is about 10 lm, inwhich the lamellar a-Al phase is 0.41 lm thick. The Fe-rich intermetallic compound exhibits acompact morphology and is less than 2 lm with a composition of 1.62 at. pct Si, 3.94 at. pct Fe,and 2.31 at. pct Mn. A solute-enriched circular band is always observed parallel to the surface ofthe casting. The band zone separates the outer skin region from the central region of the casting.The solute concentration is consistent in the skin region and shows a general drop toward thecenter inside the band for Mg and Si. The peak of the solute enrichment in the band zone ismuch higher than the nominal composition of the alloy. The die casting exhibits a combinationof brittle and ductile fracture. There is no significant difference on the fracture morphology inthe three regions. The band zone is not significantly detrimental in terms of the fracturemechanism in the die casting. Calculations using the Mullins and Sekerka stability criterionreveal that the solidification of the primary a-Al phase inside the die cavity has been completedbefore the spherical a-Al globules begin to lose their stability, but the a-Al grains formed in theshot sleeve exceed the limit of spherical growth and therefore exhibit a dendritic morphology.
DOI: 10.1007/s11661-013-1663-5 The Minerals, Metals & Materials Society and ASM International 2013
HIGH-PRESSURE die casting (HPDC) is one of themost popular manufacturing processes used in thecasting industry. The attractiveness of HPDC is itsability to make near net-shape parts with tight toler-ances, requiring little or no machining.[1,2] HPDCcastings often have low ductility and are used fornonstructural applications. However, they have beenattracting increased interest in the products of structuralapplications, particularly in transportation such asautomotive markets because of the driving force interms of weight savings leading to improved fueleconomy.[3,4] An extensive range of aluminum HPDCparts are used in the automotive industry, which includetransmission housings, cylinder heads, inlet manifolds,engine sumps, brackets, heat sinks, stators, as well as fordecorative trim items.[5,6] Moreover, an increasing trendin replacing steel parts with the lighter aluminum partshas seen aluminum HPDC parts being used extensively
in other automotive areas. One of the significantdevelopments in recent years has been their applicationin aluminum car body structures.[3,7,8] Unique mechan-ical properties are required for this specific application.For example, the ductility of aluminum components forcar body structures requires thin wall die castings withat least 15 pct of elongation. To achieve the requiredelongation, several critical aspects need to be preciselycontrolled during manufacturing which include anoptimized alloy composition, low level of gas andimpurities in melt before solidification, minimized defectlevels, and an optimized microstructure in the castings.These are associated partially or completely with thesolidification of the castings.It has been found that Al-Mg-Si-based alloys are
capable of providing high ductility and an excellentcombination of mechanical properties for die castings inthe as-cast state. However, the diecast Al-Mg (-Si)-based alloys are known to have high solidificationshrinkage which, therefore, increases the difficulty ofproducing castings with high integrity.[10,11] As such, themicrostructural evolution and the related control duringsolidification are becoming very important for achievingenhanced mechanical properties of the Al-Mg-Si alloy.The solidification of Al-Mg (-Si)-based alloys has been
the subject of many studies, but most of them fall into thecategory of wrought alloys[12,13] or high silicon (>5 wt pctSi) and low magnesium (
process. Previous studies were rather limited in describingthe solidification and microstructural evolution of highmagnesium (>4 wt pct) and silicon (>1.5 wt pct) cast alloysin HPDC process. Otarawanna et al. studied themicrostructural formation of AlSi4MgMn and AlMg5-Si2Mn castings and found that the salient as-cast micro-structural features were similar for both alloys in terms ofthe externally solidified crystals, defect bands, surfacelayer, grain size and distribution, porosity, and hot tears.Jie et al. investigated the microstructure of Al-21.6 wtpct Mg alloy solidified under high pressure inside acylindrical container at a pressure up to 2 GPa. Theyfound that the amount of b-Al3Mg2 phase decreased withthe increasing pressure, and a supersaturated Al(Mg) solidsolutionwas formed at 2 GPa.Kimura et al. studied theeffect of grain refiner and grain size on the crackingsusceptibility ofAl-4.5wt pctMgdiecast alloy.They foundthat the addition of 0.08 wt pct Ti and 0.016 wt pct B couldachieve significant grain refinement and, therefore, itsuppressed cracking formation in Al-Mg die castings.Recently, the authors investigated the effect of mainalloying elements on the mechanical properties of Al-Mg-Si diecast alloy and optimized the composition and castingprocess to satisfy the requirement of strength and ductil-ity. In HPDC process, the melt is injected into the diecavity under high speed (30 through 50 m/s ingate velocityfor aluminum alloys), and solidified under high pressure(up to 200 MPa in the die cavity) and high cooling rate (upto 103 K/s). This results in unique solidification behav-ior and offers a fundamental difference to other castingprocesses. Therefore, theoretical understanding of thesolidification process and microstructural evolution inHPDC is important for improving the process itself,microstructural control, and the mechanical properties.Moreover, defect formation is closely related to thesolidification and microstructure of the castings. This isparticularly important in determining the mechanicalproperties of ductile diecast aluminum alloys.
In the current study, investigation of the solidificationprocess andmicrostructural evolutionof ductile aluminumalloy has been carried out using HPDC process. Thesolidification behavior in the shot sleeve and in the diecavity was examined for the formation of the primary a-Alphase, eutectic phase, and Fe-rich intermetallics in Al-5 wtpct Mg-1.5 wt pct Si-0.6 wt pct Mn-0.2 wt pct Ti(abbreviated as AlMgSi hereafter) alloy. The morphol-ogy, size, and size distribution of the primary a-Al phasewere characterized under different solidification condi-tions. The phases formed in the different stages ofsolidification were identified and quantified. In the discus-sion, the growth morphology of the primary a-Al phaseformed in the shot sleeve and in the die cavitywas analyzedusing the MullinsSekerka instability theory. JacksonHunt theory was also used to calculate the growth rate ofAl-Mg2Si eutectic phase during solidification.
Commercial grade ingots of pure aluminum, puremagnesium, Al-15 wt pct Si, Al-20 wt pct Mn, and Al-10wt pct Timaster alloyswere used as basematerials. Each ofthem was supplied at a specified composition with known
industrial purity. During experiments, each element wasweighed to a specified ratio with an allowance for burningloss during melting. Batches of 6 through 10 kg weremelted in a claygraphite crucible using an electricresistance furnace at 1003 K (730 C). The melt wasthoroughly stirred to ensure complete dissolution andhomogenization. For all the experiments, the melt wassubjected to fluxing and degassing using commerciallyavailable fluxes andN2. TheN2 degassing lasted 3 minuteswith a granular flux covering the surface of themelt. Then,the melt was held at 973 K (700 C) for 20 minutes beforetaking a sample for composition measurement.A /40960mm cylindrical casting was made in a steel
mould for composition analysis. The cylindrical castingwas cut across the diameter at 15 mm from the bottomand ground to 800 grit. The composition measurementswere conducted with an optical mass spectrometer, inwhich five spark analyses were performed, and theaverage value was taken as the actual chemical compo-sition of the alloy.After compositional analysis and skimming, the melt
was manually dosed and subsequently released into theshot sleeve of a 2800-kN cold chamber HPDC machinefor casting under an optimized casting condition. Thetemperature of the die block was controlled at 484 K(211 C) and the temperature of shot sleeve was con-trolled at 423 K (150 C) during casting. The pouringtemperature of the melt was 923 K 5 K (650 5 C)measured by a K-type thermocouple. The diecastsamples for tensile tests were schematically shown inFigure 1, which were designed according to the specifi-cation defined in ASTM B557-06.The samples for microstructural evaluation were
taken from the middle of the tensile test bar, andexamined using a Zeiss optical microscope (OM) withquantitative metallography. All metallographic sampleswere prepared by a standard technique. The grain size,volume fraction, and the shape factor of the solid phasewere measured using an AxioVision 4.3 Quantimetdigital image analysis system. Five differe